data_blue-crystal 
 
_audit_creation_method            SHELXL-97
_chemical_name_systematic
;
 ?
;
_chemical_name_common             'gelosaite (Kingsgate)'
_chemical_melting_point           ?
_chemical_formula_moiety          ?
_chemical_formula_sum
 'Bi Mo2.38 O9'
_chemical_formula_weight          581.80
 
loop_
 _atom_type_symbol
 _atom_type_description
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 'Bi'  'Bi'  -4.1077  10.2566
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Mo'  'Mo'  -1.6832   0.6857
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'O'  'O'   0.0106   0.0060
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 
_symmetry_cell_setting            monoclinic
_symmetry_space_group_name_H-M    P2(1)/n
 
loop_
 _symmetry_equiv_pos_as_xyz
 'x, y, z'
 '-x+1/2, y+1/2, -z+1/2'
 '-x, -y, -z'
 'x-1/2, -y-1/2, z-1/2'
 
_cell_length_a                    5.837(3)
_cell_length_b                    9.040(5)
_cell_length_c                    13.904(7)
_cell_angle_alpha                 90.00
_cell_angle_beta                  100.640(8)
_cell_angle_gamma                 90.00
_cell_volume                      721.0(6)
_cell_formula_units_Z             4
_cell_measurement_temperature     293(2)
_cell_measurement_reflns_used     1687
_cell_measurement_theta_min       2.70
_cell_measurement_theta_max       28.37
 
_exptl_crystal_description        plate
_exptl_crystal_colour             blue-green
_exptl_crystal_size_max           0.15
_exptl_crystal_size_mid           0.10
_exptl_crystal_size_min           0.02
_exptl_crystal_density_meas       ?
_exptl_crystal_density_diffrn     5.360
_exptl_crystal_density_method     'not measured'
_exptl_crystal_F_000              1021
_exptl_absorpt_coefficient_mu     28.431
_exptl_absorpt_correction_type    empirical
_exptl_absorpt_correction_T_min   ?
_exptl_absorpt_correction_T_max   ?
_exptl_absorpt_process_details    'SORTAV (Blessing, 1995)'
 
_exptl_special_details
;
 ?
;
 
_diffrn_ambient_temperature       293(2)
_diffrn_radiation_wavelength      0.71073
_diffrn_radiation_type            MoK\a
_diffrn_radiation_source          'fine-focus sealed tube'
_diffrn_radiation_monochromator   graphite
_diffrn_measurement_device_type   'Bruker SMART diffractometer'
_diffrn_measurement_method        'phi and omega scans'
_diffrn_detector_area_resol_mean  'CCD area detector'
_diffrn_standards_number          ?
_diffrn_standards_interval_count  ?
_diffrn_standards_interval_time   ?
_diffrn_standards_decay_%         ?
_diffrn_reflns_number             1687
_diffrn_reflns_av_R_equivalents   0.0000
_diffrn_reflns_av_sigmaI/netI     0.0515
_diffrn_reflns_limit_h_min        -7
_diffrn_reflns_limit_h_max        7
_diffrn_reflns_limit_k_min        0
_diffrn_reflns_limit_k_max        11
_diffrn_reflns_limit_l_min        0
_diffrn_reflns_limit_l_max        18
_diffrn_reflns_theta_min          2.70
_diffrn_reflns_theta_max          28.37
_reflns_number_total              1687
_reflns_number_gt                 1356
_reflns_threshold_expression      >2sigma(I)
 
_computing_data_collection        'Bruker SMART'
_computing_cell_refinement        'Bruker SMART'
_computing_data_reduction         'Bruker SAINT'
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1997)'
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics     ?
_computing_publication_material   ?
 
_refine_special_details
;
 Refinement of F² against ALL reflections.  The weighted R-factor wR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, with F set to zero for negative F². The threshold expression of
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about twice as large as those based on F, and R-
 factors based on ALL data will be even larger.
;
 
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_matrix_type            full
_refine_ls_weighting_scheme       calc
_refine_ls_weighting_details
 'calc w=1/[σ²(Fo²)+(0.1234P)²+64.6300P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary      direct
_atom_sites_solution_secondary    difmap
_atom_sites_solution_hydrogens    geom
_refine_ls_hydrogen_treatment     none
_refine_ls_extinction_method      none
_refine_ls_extinction_coef        ?
_refine_ls_number_reflns          1687
_refine_ls_number_parameters      60
_refine_ls_number_restraints      0
_refine_ls_R_factor_all           0.0893
_refine_ls_R_factor_gt            0.0757
_refine_ls_wR_factor_ref          0.2115
_refine_ls_wR_factor_gt           0.1972
_refine_ls_goodness_of_fit_ref    1.101
_refine_ls_restrained_S_all       1.101
_refine_ls_shift/su_max           0.000
_refine_ls_shift/su_mean          0.000
 
loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_U_iso_or_equiv
 _atom_site_adp_type
 _atom_site_occupancy
 _atom_site_symmetry_multiplicity
 _atom_site_calc_flag
 _atom_site_refinement_flags
 _atom_site_disorder_assembly
 _atom_site_disorder_group
Bi Bi 0.09774(12) 0.91673(8) 0.39388(5) 0.0061(2) Uani 1 1 d . . .
Mo1 Mo -0.1338(3) 1.10259(18) 0.15759(12) 0.004 Uiso 1 1 d . . .
Mo2 Mo -0.3671(3) 1.22273(18) 0.34101(11) 0.0050(4) Uiso 1 1 d . . .
Mo3 Mo -0.365(2) 0.9539(16) 0.3392(10) 0.005(3) Uiso 0.12 1 d P . .
Mo4 Mo 0.0967(10) 1.2611(7) 0.3940(4) 0.0054(11) Uiso 0.27 1 d P . .
OW1 O -0.040(3) 1.4169(16) 0.3428(11) 0.011(3) Uiso 1 1 d . . .
O2 O -0.248(2) 1.0920(14) 0.0328(10) 0.005(3) Uiso 1 1 d . . .
O3 O -0.603(3) 1.1060(16) 0.3356(11) 0.012(3) Uiso 1 1 d . . .
O4 O -0.366(2) 1.2400(16) 0.1893(9) 0.006(2) Uiso 1 1 d . . .
O5 O -0.249(2) 1.2441(16) 0.4664(9) 0.005(2) Uiso 1 1 d . . .
O7 O 0.018(2) 0.9149(14) 0.1841(10) 0.007(3) Uiso 1 1 d . . .
O8 O -0.134(2) 1.0856(14) 0.3124(10) 0.004 Uiso 1 1 d . . .
O9 O 0.101(3) 1.2196(17) 0.1662(12) 0.017(3) Uiso 1 1 d . . .
OH O -0.184(3) 0.9136(15) 0.4795(10) 0.008(3) Uiso 1 1 d . . .
 
 
_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
 
loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_distance
 _geom_bond_site_symmetry_2
 _geom_bond_publ_flag
Bi OH 2.202(14) . ?
Bi O8 2.208(13) . ?
Bi O4 2.266(14) 2_445 ?
Bi OH 2.319(14) 3_576 ?
Bi O5 2.456(13) 3_576 ?
Bi O3 2.674(15) 1_655 ?
Bi Mo3 2.690(14) . ?
Bi O9 2.739(16) 2_545 ?
Bi Mo4 3.113(7) . ?
Bi Mo3 3.376(14) 1_655 ?
Bi Bi 3.6769(19) 3_576 ?
Mo1 O9 1.719(16) . ?
Mo1 O2 1.743(14) . ?
Mo1 O7 1.919(13) . ?
Mo1 O4 1.950(13) . ?
Mo1 O8 2.157(14) . ?
Mo1 OW1 2.537(15) 2_445 ?
Mo1 Mo3 3.176(15) 2_455 ?
Mo1 Mo2 3.289(3) . ?
Mo2 O3 1.726(16) . ?
Mo2 O5 1.763(12) . ?
Mo2 O8 1.937(13) . ?
Mo2 O7 1.950(13) 2_455 ?
Mo2 O4 2.115(13) . ?
Mo2 Mo3 2.430(15) . ?
Mo2 OW1 2.589(15) . ?
Mo2 Mo4 2.694(6) . ?
Mo3 O8 1.889(19) . ?
Mo3 O3 1.95(2) . ?
Mo3 OH 2.07(2) . ?
Mo3 O4 2.43(2) 2_445 ?
Mo3 OW1 2.51(2) 2_445 ?
Mo3 O9 2.52(2) 2_445 ?
Mo3 Mo1 3.176(15) 2_445 ?
Mo3 Bi 3.376(14) 1_455 ?
Mo4 OW1 1.708(16) . ?
Mo4 O8 2.246(14) . ?
Mo4 OH 2.349(15) 3_576 ?
Mo4 O2 2.380(15) 4_686 ?
Mo4 O5 2.419(13) . ?
Mo4 O3 2.494(16) 1_655 ?
OW1 Mo3 2.51(2) 2_455 ?
O2 Mo4 2.380(15) 4_585 ?
O3 Mo4 2.494(16) 1_455 ?
O3 Bi 2.674(15) 1_455 ?
O4 Bi 2.266(14) 2_455 ?
O4 Mo3 2.43(2) 2_455 ?
O5 Bi 2.456(13) 3_576 ?
O7 Mo2 1.950(13) 2_445 ?
O9 Mo3 2.52(2) 2_455 ?
O9 Bi 2.739(16) 2 ?
OH Bi 2.319(14) 3_576 ?
OH Mo4 2.349(15) 3_576 ?
 
loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_3
 _geom_angle_publ_flag
OH Bi O8 80.7(5) . . ?
OH Bi O4 80.4(5) . 2_445 ?
O8 Bi O4 88.6(5) . 2_445 ?
OH Bi OH 71.2(6) . 3_576 ?
O8 Bi OH 87.6(5) . 3_576 ?
O4 Bi OH 151.6(5) 2_445 3_576 ?
OH Bi O5 76.1(5) . 3_576 ?
O8 Bi O5 155.7(5) . 3_576 ?
O4 Bi O5 94.6(5) 2_445 3_576 ?
OH Bi O5 78.2(5) 3_576 3_576 ?
OH Bi O3 140.1(5) . 1_655 ?
O8 Bi O3 76.9(5) . 1_655 ?
O4 Bi O3 131.1(5) 2_445 1_655 ?
OH Bi O3 75.2(5) 3_576 1_655 ?
O5 Bi O3 117.4(5) 3_576 1_655 ?
OH Bi Mo3 48.9(5) . . ?
O8 Bi Mo3 44.0(5) . . ?
O4 Bi Mo3 58.1(5) 2_445 . ?
OH Bi Mo3 101.4(5) 3_576 . ?
O5 Bi Mo3 119.5(4) 3_576 . ?
O3 Bi Mo3 120.8(5) 1_655 . ?
OH Bi O9 137.9(5) . 2_545 ?
O8 Bi O9 131.3(5) . 2_545 ?
O4 Bi O9 75.0(5) 2_445 2_545 ?
OH Bi O9 126.8(5) 3_576 2_545 ?
O5 Bi O9 72.5(4) 3_576 2_545 ?
O3 Bi O9 80.3(5) 1_655 2_545 ?
Mo3 Bi O9 131.5(5) . 2_545 ?
OH Bi Mo4 90.6(4) . . ?
O8 Bi Mo4 46.2(4) . . ?
O4 Bi Mo4 134.8(4) 2_445 . ?
OH Bi Mo4 48.6(4) 3_576 . ?
O5 Bi Mo4 126.3(3) 3_576 . ?
O3 Bi Mo4 50.4(3) 1_655 . ?
Mo3 Bi Mo4 82.7(3) . . ?
O9 Bi Mo4 130.7(3) 2_545 . ?
OH Bi Mo3 160.2(4) . 1_655 ?
O8 Bi Mo3 108.7(4) . 1_655 ?
O4 Bi Mo3 116.5(4) 2_445 1_655 ?
OH Bi Mo3 91.4(4) 3_576 1_655 ?
O5 Bi Mo3 91.4(4) 3_576 1_655 ?
O3 Bi Mo3 35.2(4) 1_655 1_655 ?
Mo3 Bi Mo3 148.2(5) . 1_655 ?
O9 Bi Mo3 47.3(4) 2_545 1_655 ?
Mo4 Bi Mo3 84.4(3) . 1_655 ?
OH Bi Bi 36.7(4) . 3_576 ?
O8 Bi Bi 83.0(4) . 3_576 ?
O4 Bi Bi 117.0(3) 2_445 3_576 ?
OH Bi Bi 34.5(4) 3_576 3_576 ?
O5 Bi Bi 74.1(3) 3_576 3_576 ?
O3 Bi Bi 107.3(3) 1_655 3_576 ?
Mo3 Bi Bi 74.4(3) . 3_576 ?
O9 Bi Bi 145.3(3) 2_545 3_576 ?
Mo4 Bi Bi 65.75(10) . 3_576 ?
Mo3 Bi Bi 125.4(2) 1_655 3_576 ?
O9 Mo1 O2 104.9(7) . . ?
O9 Mo1 O7 101.3(7) . . ?
O2 Mo1 O7 102.8(6) . . ?
O9 Mo1 O4 99.9(7) . . ?
O2 Mo1 O4 96.1(6) . . ?
O7 Mo1 O4 146.8(6) . . ?
O9 Mo1 O8 96.9(6) . . ?
O2 Mo1 O8 156.7(6) . . ?
O7 Mo1 O8 80.2(5) . . ?
O4 Mo1 O8 72.0(5) . . ?
O9 Mo1 OW1 174.9(6) . 2_445 ?
O2 Mo1 OW1 79.2(6) . 2_445 ?
O7 Mo1 OW1 74.6(5) . 2_445 ?
O4 Mo1 OW1 82.5(5) . 2_445 ?
O8 Mo1 OW1 79.5(5) . 2_445 ?
O9 Mo1 Mo3 52.2(6) . 2_455 ?
O2 Mo1 Mo3 93.9(5) . 2_455 ?
O7 Mo1 Mo3 152.1(5) . 2_455 ?
O4 Mo1 Mo3 50.0(5) . 2_455 ?
O8 Mo1 Mo3 93.2(4) . 2_455 ?
OW1 Mo1 Mo3 131.2(4) 2_445 2_455 ?
O9 Mo1 Mo2 100.5(5) . . ?
O2 Mo1 Mo2 130.7(5) . . ?
O7 Mo1 Mo2 112.7(4) . . ?
O4 Mo1 Mo2 37.7(4) . . ?
O8 Mo1 Mo2 34.3(4) . . ?
OW1 Mo1 Mo2 78.6(3) 2_445 . ?
Mo3 Mo1 Mo2 69.9(2) 2_455 . ?
O3 Mo2 O5 105.9(7) . . ?
O3 Mo2 O8 100.7(6) . . ?
O5 Mo2 O8 96.4(6) . . ?
O3 Mo2 O7 101.9(7) . 2_455 ?
O5 Mo2 O7 99.3(6) . 2_455 ?
O8 Mo2 O7 147.7(6) . 2_455 ?
O3 Mo2 O4 98.6(6) . . ?
O5 Mo2 O4 154.8(6) . . ?
O8 Mo2 O4 73.2(6) . . ?
O7 Mo2 O4 80.8(6) 2_455 . ?
O3 Mo2 Mo3 52.6(6) . . ?
O5 Mo2 Mo3 96.8(6) . . ?
O8 Mo2 Mo3 49.7(5) . . ?
O7 Mo2 Mo3 153.1(5) 2_455 . ?
O4 Mo2 Mo3 93.6(5) . . ?
O3 Mo2 OW1 174.7(6) . . ?
O5 Mo2 OW1 76.3(6) . . ?
O8 Mo2 OW1 83.7(5) . . ?
O7 Mo2 OW1 72.9(5) 2_455 . ?
O4 Mo2 OW1 79.8(5) . . ?
Mo3 Mo2 OW1 132.3(5) . . ?
O3 Mo2 Mo4 147.6(5) . . ?
O5 Mo2 Mo4 61.6(4) . . ?
O8 Mo2 Mo4 55.2(4) . . ?
O7 Mo2 Mo4 109.4(4) 2_455 . ?
O4 Mo2 Mo4 94.4(4) . . ?
Mo3 Mo2 Mo4 97.2(4) . . ?
OW1 Mo2 Mo4 37.7(4) . . ?
O3 Mo2 Mo1 101.9(5) . . ?
O5 Mo2 Mo1 131.3(4) . . ?
O8 Mo2 Mo1 38.9(4) . . ?
O7 Mo2 Mo1 113.2(4) 2_455 . ?
O4 Mo2 Mo1 34.3(4) . . ?
Mo3 Mo2 Mo1 70.0(3) . . ?
OW1 Mo2 Mo1 79.7(3) . . ?
Mo4 Mo2 Mo1 73.46(13) . . ?
O8 Mo3 O3 94.8(9) . . ?
O8 Mo3 OH 92.2(8) . . ?
O3 Mo3 OH 112.7(9) . . ?
O8 Mo3 Mo2 51.5(5) . . ?
O3 Mo3 Mo2 44.8(5) . . ?
OH Mo3 Mo2 99.7(7) . . ?
O8 Mo3 O4 91.7(7) . 2_445 ?
O3 Mo3 O4 166.3(9) . 2_445 ?
OH Mo3 O4 79.1(7) . 2_445 ?
Mo2 Mo3 O4 143.1(7) . 2_445 ?
O8 Mo3 OW1 85.3(7) . 2_445 ?
O3 Mo3 OW1 92.6(8) . 2_445 ?
OH Mo3 OW1 154.7(9) . 2_445 ?
Mo2 Mo3 OW1 98.2(6) . 2_445 ?
O4 Mo3 OW1 75.8(6) 2_445 2_445 ?
O8 Mo3 O9 158.6(9) . 2_445 ?
O3 Mo3 O9 102.1(8) . 2_445 ?
OH Mo3 O9 93.5(8) . 2_445 ?
Mo2 Mo3 O9 146.8(7) . 2_445 ?
O4 Mo3 O9 69.2(6) 2_445 2_445 ?
OW1 Mo3 O9 80.8(6) 2_445 2_445 ?
O8 Mo3 Bi 54.3(5) . . ?
O3 Mo3 Bi 140.3(8) . . ?
OH Mo3 Bi 53.2(5) . . ?
Mo2 Mo3 Bi 97.4(5) . . ?
O4 Mo3 Bi 52.2(4) 2_445 . ?
OW1 Mo3 Bi 106.9(6) 2_445 . ?
O9 Mo3 Bi 114.7(7) 2_445 . ?
O8 Mo3 Mo1 129.5(7) . 2_445 ?
O3 Mo3 Mo1 134.6(8) . 2_445 ?
OH Mo3 Mo1 79.2(6) . 2_445 ?
Mo2 Mo3 Mo1 178.5(6) . 2_445 ?
O4 Mo3 Mo1 37.8(4) 2_445 2_445 ?
OW1 Mo3 Mo1 83.1(5) 2_445 2_445 ?
O9 Mo3 Mo1 32.6(4) 2_445 2_445 ?
Bi Mo3 Mo1 82.8(4) . 2_445 ?
O8 Mo3 Bi 146.6(8) . 1_455 ?
O3 Mo3 Bi 52.3(6) . 1_455 ?
OH Mo3 Bi 95.9(6) . 1_455 ?
Mo2 Mo3 Bi 95.2(4) . 1_455 ?
O4 Mo3 Bi 121.6(6) 2_445 1_455 ?
OW1 Mo3 Bi 100.0(6) 2_445 1_455 ?
O9 Mo3 Bi 53.0(4) 2_445 1_455 ?
Bi Mo3 Bi 148.2(5) . 1_455 ?
Mo1 Mo3 Bi 83.9(3) 2_445 1_455 ?
OW1 Mo4 O8 100.5(7) . . ?
OW1 Mo4 OH 152.4(7) . 3_576 ?
O8 Mo4 OH 86.0(5) . 3_576 ?
OW1 Mo4 O2 87.5(6) . 4_686 ?
O8 Mo4 O2 155.0(5) . 4_686 ?
OH Mo4 O2 76.7(5) 3_576 4_686 ?
OW1 Mo4 O5 82.2(6) . . ?
O8 Mo4 O5 72.4(5) . . ?
OH Mo4 O5 74.2(5) 3_576 . ?
O2 Mo4 O5 85.3(5) 4_686 . ?
OW1 Mo4 O3 129.1(7) . 1_655 ?
O8 Mo4 O3 80.2(5) . 1_655 ?
OH Mo4 O3 78.3(5) 3_576 1_655 ?
O2 Mo4 O3 113.1(5) 4_686 1_655 ?
O5 Mo4 O3 142.1(6) . 1_655 ?
OW1 Mo4 Mo2 67.9(5) . . ?
O8 Mo4 Mo2 45.1(4) . . ?
OH Mo4 Mo2 100.8(4) 3_576 . ?
O2 Mo4 Mo2 120.4(4) 4_686 . ?
O5 Mo4 Mo2 39.9(3) . . ?
O3 Mo4 Mo2 124.7(4) 1_655 . ?
OW1 Mo4 Bi 145.6(6) . . ?
O8 Mo4 Bi 45.2(4) . . ?
OH Mo4 Bi 47.8(4) 3_576 . ?
O2 Mo4 Bi 123.9(4) 4_686 . ?
O5 Mo4 Bi 86.5(4) . . ?
O3 Mo4 Bi 55.7(4) 1_655 . ?
Mo2 Mo4 Bi 82.71(17) . . ?
Mo4 OW1 Mo3 121.9(8) . 2_455 ?
Mo4 OW1 Mo2 74.5(5) . . ?
Mo3 OW1 Mo2 93.2(6) 2_455 . ?
Mo1 O2 Mo4 142.7(7) . 4_585 ?
Mo2 O3 Mo3 82.6(8) . . ?
Mo2 O3 Mo4 104.2(7) . 1_455 ?
Mo3 O3 Mo4 158.3(9) . 1_455 ?
Mo2 O3 Bi 159.8(9) . 1_455 ?
Mo3 O3 Bi 92.5(7) . 1_455 ?
Mo4 O3 Bi 74.0(4) 1_455 1_455 ?
Mo1 O4 Mo2 107.9(6) . . ?
Mo1 O4 Bi 135.0(6) . 2_455 ?
Mo2 O4 Bi 116.8(6) . 2_455 ?
Mo1 O4 Mo3 92.2(6) . 2_455 ?
Mo2 O4 Mo3 108.9(6) . 2_455 ?
Bi O4 Mo3 69.7(5) 2_455 2_455 ?
Mo2 O5 Mo4 78.5(5) . . ?
Mo2 O5 Bi 137.3(7) . 3_576 ?
Mo4 O5 Bi 99.3(5) . 3_576 ?
Mo1 O7 Mo2 125.1(7) . 2_445 ?
Mo3 O8 Mo2 78.8(7) . . ?
Mo3 O8 Mo1 111.9(8) . . ?
Mo2 O8 Mo1 106.8(6) . . ?
Mo3 O8 Bi 81.7(6) . . ?
Mo2 O8 Bi 136.4(7) . . ?
Mo1 O8 Bi 116.7(6) . . ?
Mo3 O8 Mo4 136.8(8) . . ?
Mo2 O8 Mo4 79.8(5) . . ?
Mo1 O8 Mo4 110.1(6) . . ?
Bi O8 Mo4 88.7(5) . . ?
Mo1 O9 Mo3 95.2(8) . 2_455 ?
Mo1 O9 Bi 158.1(9) . 2 ?
Mo3 O9 Bi 79.8(6) 2_455 2 ?
Mo3 OH Bi 77.9(6) . . ?
Mo3 OH Bi 126.9(8) . 3_576 ?
Bi OH Bi 108.8(6) . 3_576 ?
Mo3 OH Mo4 145.7(8) . 3_576 ?
Bi OH Mo4 109.4(6) . 3_576 ?
Bi OH Mo4 83.6(5) 3_576 3_576 ?
 
_diffrn_measured_fraction_theta_max    0.933
_diffrn_reflns_theta_full              28.37
_diffrn_measured_fraction_theta_full   0.933
_refine_diff_density_max   14.749
_refine_diff_density_min   -6.252
_refine_diff_density_rms    0.950
